Tribological properties of Cr- and Ti-doped MoS2 composite coatings under different
Xing-zhao Ding a, ⁎, X.T. Zeng a , X.Y. He b , Z. Chen b
a Singapore Institute of Manufacturing Technology, 71 Nanyang Drive, Singapore 638075, Singapore
b School of Materials Science and Engineering, Nanyang Technological University, Nanyang Avenue, Singapore 639798, Singapore
Received 6 May 2010
Accepted in revised form 19 June 2010
Available online 1 July 2010
Physical vapor deposition
MoS 2-metal composite coatings
Many industrial and engineering applications require two surfaces
to slide over one another, resulting in friction and wear. Examples
include various cutting and forming tools, and generic wear
components (gears, bearings, engine parts, etc.) as well. Nowadays,
surface coating has increasingly become a routine step in tools'
manufacturing industry. These tribological coatings can effectively
reduce friction, improve wear resistance, increase tool lifetime,
improve tool performance, and enhance the productivity as well.
Practically, two main properties are fundamental to tool coatings:
high hardness and lubricity. The higher hardness of the hard coatings
gives the tools much greater protection against abrasive wear, while
the lower coefficient of friction means that the tool will work with less
force due to the reduced resistance.
Transition metal nitrides, carbides and carbonitrides, include TiN,
TiCN, TiAlN, CrN-based, and ZrN-based coatings have proved to be
very successful and are widely used in improving the performance of
⁎ Corresponding author. Tel.: +65 67938528; fax: +65 67922779.
E-mail address: xzding@SIMTech.a-star.edu.sg (X. Ding).
0257-8972/$ – see front matter © 2010 Elsevier B.V. All rights reserved.
Surface & Coatings Technology 205 (2010) 224–231
Contents lists available at ScienceDirect
Surface & Coatings Technology
journal homepage: www.elsevier.com/locate/surfcoat
Solid-lubricant MoS2 coatings have been successfully applied in high vacuum and aerospace environments.
However, these coatings are very sensitive to water vapor and not suitable for applications in moist
environments. In this work, Cr- and T-doped MoS2 composite coatings were developed. The results
demonstrated that these composite coatings are promising for applications in high humidity environments.
MoS2–Cr and MoS2–Ti composite coatings with different Cr or Ti content were deposited on high speed steel
substrate by unbalanced magnetron sputtering. The composition, microstructure, and mechanical properties
of the as-deposited MoS2-metal composite coatings were analyzed by energy dispersive analysis of X-ray
(EDX), X-ray diffraction (XRD), and nanoindentation experiments. The tribological properties of the coatings
were evaluated against an alumina ball under different relative humidity atmosphere using a ball-on-disc
tribometer. The MoS2–Cr and MoS2–Ti coatings showed a maximum hardness of 7.5 GPa and 8.4 GPa at a
dopant content of 16.6 at.% Cr or 20.2 at.% Ti, respectively. The tribological test results showed that, with a
small amount of Cr and/or Ti doping, the tribological properties of MoS2 coatings under humid atmosphere
could be significantly improved. The optimum doping level was found to be around 10 at.% for both MoS2–Cr
coatings and MoS2–Ti coatings to show the best tribological properties, with both the lowest friction
coefficient and wear rate. The excellent tribological properties of the MoS2–Cr and MoS2–Ti coatings with an
appropriate metal doping level in moist atmosphere are found due to their ability to form stable transfer
layer on the surface of the counterbody, which supplies lubrication for the contact surface.
© 2010 Elsevier B.V. All rights reserved.
cutting and forming tools, because of their high hardness, wear
resistance, and chemical stability . However, these conventional
hard coatings generally exhibit a high coefficient of friction and cause
abrasive wear on the opposing surface. Therefore, lubricants are still
required in many practical applications.
For centuries, liquid lubricants were used to limit the contact
pressure and reduce the temperature produced by friction. But, in many
cases, for instance in a vacuum environment, at high temperature
application conditions, for food and medical apparatus, and so on, the
presence of liquid lubricants is not recommended or forbidden for
contamination and/or safety reasons. As an alternative, solid lubricants
are often used in many industrial applications , which cause less or no
contamination compared to liquid lubricants. Solid lubricants are
appealing in promoting dry machining to avoid environmentally
harmful liquid lubricants either fully or partially. MoS2 is the most
widely used lamellar compound solid lubricant.
Since the pioneer work of Spalvins , solid-lubricant MoS2 coatings
produced by physical vapor deposition (PVD) processes have been
successfully applied in high vacuum and aerospace environments [4,5],
e.g. bearings and gears in artificial satellites, for many years. The solid
lubricant coating reduces the friction and protects both its own surface
and the opposing surface in contrast to the conventional hard coatings.
Fig. 1. Cr (a) and Ti (b) content in the as-deposited MoS2–Cr or MoS2–Ti composite
coatings as a function of DC sputtering current applied on the Cr or Ti target. Typical
spectra of the coatings are shown in the inserts.
X. Ding et al. / Surface & Coatings Technology 205 (2010) 224–231
In normal terrestrial atmosphere, however, MoS2 is prone to water
adsorption from air because of its hygroscopic property. Hence, it is very
sensitive to water vapor [5–7], resulting in poor tribological properties,
including increased friction coefficient, degraded wear resistance, and
reduced lifetime. Therefore, MoS2 coatings are not suitable for practical
applications in moist environments.
In the past two decades, co-sputtered MoS2-metal composite
coatings or MoS2-metal multilayered coatings [8–20] have been widely
reported by many research groups to exhibit improvement in hardness,
adhesion strength, and tribological performance in air over the pure
MoS2 coatings. Particularly, among these co-deposited coatings, the
MoS2–Ti composite coatings (trade-marked by Teer Coatings Ltd as
MoST) have been intensively investigated [8–16]. The MoST
composite coatings have given excellent industrial results for a wide
range of cutting and forming tool applications at normal cutting speeds,
showing big improvements in comparison with conventional hard
coatings. Similar to the MoST composite coatings, MoS 2–Cr composite
coatings have also attracted lots of attentions [15–20]. Chromiummay
behave similarly to titanium in the MoS 2-metal composite coating
system, and in some specific applications, such as in machining brasses
and stamping of copper-based coinage, chromium is expected to give
better performance .
In this work, MoS 2–Cr and MoS 2–Ti composite coatings with
different Cr or Ti contents were deposited on high speed steel (HSS)
by unbalanced magnetron sputtering. The tribological performance of
the as-deposited coatings under different relative humidity atmosphere
was evaluated using a ball-on-disc tribometer against alumina ball.
2. Experimental details
MoS2–Cr and MoS2–Ti composite coatings, with a thickness of
around 3.5 μm, were deposited by a Teer UDP-550 unbalanced
magnetron sputtering system which has been described in detail in
our previous works [21,22]. In the bottom part of the deposition
chamber, a cryogenic-type cold trap (PolyCold System Inc., California,
USA) was installed. The temperature of the cold trap is controlled
between −105 and −115 °C during the whole process of coating
Fig. 2. XRD patterns of the as-deposited MoS 2–Cr (a) and MoS 2–Ti (b) composite coatings with different Cr or Ti content.
226 X. Ding et al. / Surface & Coatings Technology 205 (2010) 224–231
Fig. 3. Hardness of the as-deposited MoS 2–Cr (a) and MoS 2–Ti (b) composite coatings
as a function of Cr or Ti content in the coatings.
deposition. On one hand, the Polycold system is helpful for
accelerating the pumping rate of the vacuum system so as to achieve
a high level of base vacuum. Particularly, on the other hand, the
Polycold system is effective for removal of residual water vapor in the
deposition chamber, and consequently reduces oxygen contamination
in the as-deposited coatings, which is critically important for the MoS2
In this work, one elemental chromium or titanium target and two
molybdenum disulfide compound targets were used. Coating deposition
was conducted in a flowingpureAratmospherewithaworking
pressure around 0.15 Pa. All the targets were direct current (DC) power
sputtered. The sputtering current applied onto the MoS2 targets was
fixed at 0.8 A. In order to control the metal dopping level in the
as-deposited composite coatings, the DC current applied on the Cr or Ti
target was changed batch by batch. For depositing the MoS 2–Cr coatings,
the sputtering current applied on the Cr target was adjusted from 0 to
1.0 A, and correspondingly, the Cr content in the resultant coatings
changed from 0 to 33.8 at.%. While for depositing the MoS2–Ti coatings,
the sputtering current applied on the Ti target was adjusted from 0 to
2.5 A, and the Ti content in the resultant coatings changed from 0 to
29.7 at.%. Mirror-finished high speed steel (HSS) discs with a diameter
of 50 mm were used as substrates. Before loading into the vacuum
chamber, the HSS substrates were ultrasonically cleaned in a series of
alkaline solutions, washed in deionized water, dried by nitrogen gas
blowing and further dried in an oven at 100 °C. Then the precleaned
substrates were mounted on a vertical substrate holder which rotated
continuously around the central axis at a speed of 10 rpm. Prior to
coating deposition, the vacuum chamber was pumped down to
2×10 −4 Pa or lower, and the substrates were in situ cleaned with an
argon plasma at a bias of −500 V for half an hour. During deposition, a
negative pulsed direct current (PDC) bias of −70 V, with a frequency
and duration of 50 kHz and 2.0 μs respectively, was applied to the
substrates. Similar to our previous work [21,22], in order to enhance
coating adhesion onto the substrate, a multilayer structure was
constructed. It started with a Cr or Ti bonding layer (∼100 nm),
followed by a gradient Cr–MoS2 or Ti–MoS2 ramping layer (∼400 nm) in
which Cr or Ti content was decreased while MoS2 content was increased
gradually, and finished with the MoS2–Cr or MoS2–Ti composite top
layer. Even for the “pure” MoS2 coatings referred in this paper, they also
started with the Cr or Ti bonding layer and followed by the gradient
ramping layer. Only in the top layer of these “pure” MoS2 coatings, the
metal doping content is zero.
After deposition, the composition of the as-deposited coatings was
measured by energy dispersive analysis of X-rays (EDX), which is
attached to a scanning electron microscope, operating at 8 keV and
using the INCA quantitative analysis software. The microstructure of the
coatings was analyzed by X-ray diffraction (XRD) which was performed
on a Philips x-ray diffractometer in a θ–2θ scan mode using Cu K α
radiation (40 kV, 30 mA). Micro hardness of the coatings was measured
using a Nanotest 550 nanoindenter equipped with a Berbovich diamond
indenter (a three-sided pyramid), with the maximum indentation
depth around 300 nm. For each sample, eight points were measured and
the average hardness and standard deviation were obtained.
To evaluate the tribological properties of the as-deposited composite
coatings, sliding wear tests were carried out at room temperature
(∼24 °C) against an alumina ball with 9.5 mm in diameter using a
pin-on-disc tribometer (CETR UMT-2) under a normal load of 20 N. The
sliding linear speed and total sliding distance were set at 10 cm/s and
700 m, respectively. The normalized wear rate was calculated from the
preset normal load, total sliding distance, wear track diameter, and
cross-sectional area of the wear track which can be measured by a
surface profilometer. After the pin-on-disc tests, the morphology and
composition of the wear track on the coating sample and the contact
area of the alumina ball were analyzed by SEM attached with EDX. In
order to investigate the influence of humidity on the tribological
properties of the as-deposited composite coatings, wear tests were
conducted in an enclosed chamber connected with a water bubbler and
dry air supplier. The relative humidity in the testing chamber was
precisely controlled at ≤8% (will be referred as 0% or dry atmosphere in
this work), 25%, 50%, 75%, and ≥98% (will be referred as 100% or
extreme humidity atmosphere in this work), respectively.
3. Results and discussions
The Cr and Ti content in the as-deposited MoS2–Cr or MoS2–Ti
coatings are shown in Fig. 1a and b, respectively, as a function of the DC
sputtering current (ICr or ITi) applied on the Cr or Ti target. It is as
expected that Cr and Ti content increased almost linearly with the
increase of ICr or ITi. With the increase of ICr from 0 to 1.0 A, the Cr content
in the MoS 2–Cr coatings monotonously increased from 0 to around
33.8 at.%. The Ti content in the MoS2–Ti coatings increased from 0 to
29.7 at.% with the increase of I Ti from 0 to 2.5 A. The typical EDX spectra
of these coatings are shown in the inserts of the figure. No oxygen
content was detected in the as-deposited coatings, either pure MoS 2,or
MoS2–Cr or MoS2–Ti composite coatings.
Fig. 2 shows the XRD patterns of the as-deposited MoS 2–Cr and
MoS2–Ti coatings. Besides the diffraction peaks arisen from the HSS
substrate (marked as HSS in the figure), there was a evident peak at
around 2θ=34° for “pure” MoS2 coatings (Cr or Ti content in the top
layer is zero) which could be assigned to the MoS 2 (100) plane.
According to Arslane et al. , this type of coating with the basal planes
parallel to sliding direction not only supplies good lubrication property
but also is more resistant to oxidation because of the edge sites are
X. Ding et al. / Surface & Coatings Technology 205 (2010) 224–231
Fig. 4. Traces of friction coefficient of the MoS 2–Cr (left) and MoS 2–Ti (right) composite coatings during the sliding wear test against alumina under different relative humidity atmosphere.
228 X. Ding et al. / Surface & Coatings Technology 205 (2010) 224–231
Fig. 5. Variation of friction coefficient at steady stage of the MoS 2–Cr (a) and MoS 2–Ti
(b) composite coatings versus the relative humidity of the testing atmosphere.
protected. With the incorporation of the metal component, either Cr or
Ti, the MoS 2 (100) diffraction peak disappeared, and no other peaks
related to the coating material can be observed, indicating that the
composite coatings become of amorphous structure. This fact could be
attributed to the lattice distortion caused by metal incorporation.
Fig. 3 displays the hardness of MoS2–Cr and MoS2–Ti composite
coatings as a function of Cr or Ti content. The change in hardness for both
coatings showed a similar trend. In lower metal content region, the
coating hardness increased with the increase of doping content.
A maximum hardness of about 7.5 GPa or 8.4 GPa was obtained at
around 16.6 at.% Cr or 20.2 at.% Ti for the MoS 2–Cr and MoS 2–Ti coatings,
respectively. The hardness enhancement of the MoS2-metal composite
coatings can be ascribed to solid solution hardening effect, i.e. the
distortion of the MoS2 lattice caused by the incorporation of doping
metal atoms . When studying both multilayered and monolayer
co-deposited MoS2-metal composite coatings, Lince et al.  found
that the incorporation of metal components into the MoS 2 coatings led
to a denser coating structure, and thus believed that the densification
fact is responsible for the coating hardness enhancement. When the
metal doping content increased further, the coating hardness decreased
rapidly. This fact might be due to the possible formation of discrete
metallic particles .
3.1. Tribological properties
During wear testing, the friction coefficient of the wear pairs was
automatically recorded. Fig. 4 shows the traces of friction coefficient of
the MoS 2–Cr and MoS 2–Ti composite coatings in the wear tests against
alumina under different relative humidity atmosphere. For pure MoS2
Fig. 6. Comparison of the wear rate of pure MoS2 coating and the lower doped MoS2–Cr
(a) and MoS2–Ti (b) composite coatings under different relative humidity atmosphere.
coatings, the friction coefficient under dry atmosphere (RH=0%) is very
low, around 0.05. However, the pure MoS 2 coatings are very sensitive to
moisture, and their friction coefficient increased monotonously with the
increase of RH value. With a small amount of metal incorporation
(Cr content≤16.6 at.% or Ti content ≤ 15.2 at.%), the MoS2-metal
composite coatings have a similar friction coefficient with pure MoS2
under dry conditions. But these composite coatings are very stable
against moisture. Their friction coefficient remains at a very low level
(≤0.1) under various humidity conditions, except that of the
MoS2–16.6 at.%Cr and MoS2–15.2 at.%Ti coatings under the extreme
100% RH atmosphere. For the coatings with higher metal content
(Cr content≥23.5 at.% or Ti content ≥ 20.2 at.%), however, the friction
coefficient becomes very high and unstable, which results in very high
wear rate. The average friction coefficient in the relative steady stage of
the MoS 2–Cr and MoS 2–Ti coatings under different RH atmosphere is
shown in Fig. 5.
It is interesting to note that for the MoS 2–Cr coatings with higher Cr
content, the friction coefficient under dry atmosphere is very high
(∼0.8). With increasing the RH value in the testing atmosphere, the
friction coefficient was evidently reduced and a minimum friction
coefficient is obtained under a certain RH value. It was further noticed
that the higher the Cr content is in the coating, the higher RH value will
be under which the minimum friction coefficient is obtained. For the
highest Cr-doped composite coating in this work (MoS2–33.8 at% Cr),
the friction coefficient is inversely proportional to the RH value, and its
minimum friction coefficient was obtained at the extreme RH=100%
humidity condition, clearly indicating that the moisture plays a role of
lubrication for the higher Cr-doped MoS2 composite coatings. Based on
the above-mentioned experimental phenomena, it can be concluded
that for the coatings with lower Cr content (≤16.6 at.%), the MoS2 solid
lubrication plays the major role on the tribological performance of the
MoS2–Cr composite coatings. But for the higher Cr-doped coatings
(Cr content≥23.5 at.%), water vapor becomes more and more important
in determining the tribological behavior of the coatings. Similar to
the higher doped MoS 2–Cr coatings, a minimum friction coefficient was
also obtained at a certain RH for the higher doped MoS2–Ti coatings. But
the relationship between the Ti content and the RH value showing the
minimum friction coefficient was not so clear or consistent for the
MoS 2–Ti composite coatings.
Mohrbacher, et al.  once reported that the fretting behavior of
PVD TiN coatings vibrating against corundum counterbody was very
sensitive to the relative humidity in the ambient atmosphere. Fretting at
a low relative humidity is characterized by high friction coefficient
above unity. At high relative humidity, the coefficient of friction dropped
significantly down to around 0.2. It was found that during the fretting
tests, TiN coatings degraded by oxidational wear. Initially, the degraded
coating material was transferred to the corundum counterbody where it
forms a compact oxide layer having a mixed stoichiometry between TiO
and TiO 2. During further fretting, loose wear particles having a highly
defective rutile (TiO2) structure are emerging in the contact zone. The
incorporation of environmental moisture in the defective debris results
in a low shear strength layer effectively reducing the coefficient of
friction. Similarly, the high friction coefficient of the highly doped
MoS2–Cr and MoS2–Ti composite coatings in dry atmosphere might also
be ascribed to the tribo-oxidation of the Cr or Ti components. With
X. Ding et al. / Surface & Coatings Technology 205 (2010) 224–231
Fig. 7. SEM morphologies (a) of the wear scar and the EDX spectrum (b) on the contactedareaonthealuminaballafterslidingwearagainstthepureMoS 2 coating under RH=75% atmosphere.
increasing RH, the incorporation of moisture with the oxide wear debris
could form soft hydroxides with low shear strength, which resulted in a
great decrease of friction coefficient. The resultant wear surfaces would
become very smooth and available for hydro-dynamic lubrication with
Generally, the wear rate of the highly doped MoS 2-metal composite
coatings (with Cr or Ti content≥20 at.%) is very high, about two orders
in magnitude higher than that of the lower doped composite coatings, as
observed in our work. In many cases, these coatings were wore out
during the sliding wear tests. These coatings will be further investigated
in our future work. Later on in the present paper, the investigation on
the tribological properties of the MoS 2-metal composite coatings will be
focused on the lower doped coatings (i.e. with Cr content≤16.6 at.% or
Ti content≤15.2 at.%).
Fig. 6 comparesthewearrateofthepureMoS2 coatings and MoS2–Cr
(a) and MoS 2–Ti (b) coatings with lower metal content. Under dry
conditions, the wear rate of pure MoS2 coating is similar to that of the
MoS 2–9.6 at.% Cr, and evidently lower than that of the MoS 2–16.6 at.% Cr
coating. With the increase of RH value in the testing atmosphere, the wear
rate of the pure MoS 2 coating increased rapidly, while that of both the
MoS2–9.6 at.% Cr and MoS2–16.6 at.% Cr composite coatings decreased
gradually when the RH was increased up to 50% and thereafter increased
when RH was increased further. At RH=75%, the wear rate of the pure
MoS2 coating (2.2×10 −5 mm 3 /Nm) is about 30 and 7 times higher than
that of the MoS2–9.6 at.% Cr (8.0×10 −7 mm 3 /Nm) and MoS2–16.6 at.% Cr
(3.0×10 −6 mm 3 /Nm) coatings, respectively. Under all testing conditions,
Fig. 8. SEM morphologies (a) of the wear scar and the EDX spectrum (b) on the contacted area on the alumina ball after sliding wear against the MoS 2–Cr (9.6 at.%) coating under
230 X. Ding et al. / Surface & Coatings Technology 205 (2010) 224–231
Fig. 9. SEM morphologies (a) of the wear scar and the EDX spectrum (b) on the contacted area on the alumina ball after sliding wear against the MoS 2–Ti (9.5 at.%) coating under
the MoS 2–9.6 at.% Cr coating exhibited the lowest wear rate, indicating the
optimum Cr doping level for the best wear resistant MoS2–Cr coatings is
around 10 at.%.
ForboththeMoS2–9.5 at.% Ti and MoS2–15.2 at.% Ti coatings, a very
low wear rate (≤2.0×10 −7 mm 3 /Nm) was measured and this excellent
wear resistance could be remained even the relative humidity of the
testing atmosphere was increased up to 75%. The MoS 2–9.5 at.% Ti
composite coating always shows the lowest friction coefficient and wear
rate in various RH atmosphere, indicating that the optimum Ti doping
level for the best wear resistant MoS2–Ti coatings is also around 10 at.%.
Fig. 7 shows the morphology of the wear scar on the Al 2O 3 ball and
the corresponding EDX spectrum taken from the contact area after the
sliding wear test against the pure MoS 2 coating in a RH=75%
atmosphere. Only a very little amount of Mo was detected in the
contact area on the alumina ball, indicating that there was little MoS 2
transfer layer formed on the alumina ball, which is responsible for the
higher wear rate of the pure MoS 2 coatings in high humid atmosphere.
The bad tribological properties of the pure MoS2 coatings under
humidity conditions could be interpreted that the water vapor and/or
oxygen atoms go into the space between the sulphur planes, disrupt the
bonding between the plane . Thus, pure MoS 2 coating is not able to
form stable transfer layer on the counterbody.
Fig. 8 shows the morphology of the wear scar on the Al 2O 3 ball and
the corresponding EDX spectrum taken from the contact area after
sliding against the MoS2–9.6 at.% Cr composite coating in a 75% RH
atmosphere. In contrast to the case against the pure MoS2 coating,
evident Mo, S and Cr signals were detected in the contact area on the
alumina ball after sliding wear against the MoS2–9.6 at.% Cr coating,
indicating that a transfer layer composed of Mo, S and Cr was formed
on the alumina ball. The formation of this lubricious transfer layer
prevents the direct contact between the Al2O3 ball and the MoS2–Cr
coating and results in the lower wear rate of the coating. For the
MoS2–Ti composite coatings with lower Ti content, the formation of a
similar lubricious transfer layer on the alumina counterbody's contact
surface was also confirmed, as shown in Fig. 9, which leads to the
excellent wear resistance of the composite coatings.
The addition of a small amount of Cr or Ti atoms might enter the
space between the sulphur planes and prevent the water vapor entering
the coating. The lower doped MoS2–Cr or MoS2–Ti coatings still remain
the lamellar base structure of MoS 2 material, so they are able to form a
stable transfer layer and provide good tribological properties in high
humidity atmosphere. However, when the limit of the solubility
reaches, the Cr or Ti would no longer stay in the interstitial sites but
precipitate out forming a discrete metal or multilayer, bad tribological
properties would be observed.
Pure MoS 2 coatings exhibit excellent tribological properties in dry
atmosphere, but they are very sensitive to moisture. Their friction
coefficient and wear rate increased significantly with the increase of
relative humidity. With a small amount of Cr or Ti (≤16 at.%) doping, the
tribological properties of the resultant composite coatings remain
excellent even the relative humidity is increased up to 75%. When the
doping content is further increased (N20 at.%), the tribological behavior of
these composite coatings changed distictively, and their wear resistance is
greatly degraded. The optimum doping level was found to be around
10 at.% for both MoS2–Cr coatings and MoS2–Ti coatings to show the best
tribological properties, with both the lowest friction coefficient and wear
rate. The excellent tribological properties of the MoS2–Cr and MoS2–Ti
coatings with an appropriate metal doping level in moist atmosphere are
found due to their ability to form stable transfer layer on the surface of the
counterbody, which supplies lubrication for the contact surface. These
excellent tribological properties demonstrated a very promising applicability
of the MoS 2–Cr and MoS 2–Ti composite coatings in wide range
working conditions, from dry to high humidity atmospheres.
The authors would like to express their gratitude to Mr. Anthony
Yeo and Ms Liu Yuchan for their technical assistance in this work.
 H.G. Prengel, W.R. Pfouts, A.T. Santhanam, Surf. Coat. Technol. 102 (1998) 183.
 A. Erdemir, Solid lubricants and self-lubricating films, in: B. Bhushan (Ed.),
Modern Tribology Handbook, CRC Press, Boca Raton, FL, 2001, p. 787.
 T. Spalvins, ASLE Trans. 12 (1969) 36.
 T. Spalvins, J. Vac. Sci. Technol. A 5 (1987) 212.
 L.E. Pope, J.K.G. Panitz, Surf. Coat. Technol. 36 (1988) 341.
 M.R. Hilton, P.D. Fleischauer, Surf. Coat. Technol. 54/55 (1992) 435.
 C. Donnett, J.M. Martin, M.T. Le, M. Beiin, Tribol. Int. 29 (1996) 123.
 D.G. Teer, V. Bellido-Gonzales, J. Hampshire, UK Patent GB9514773.2
(19/07/1995), EU Patent 0842306.
 D.G. Teer, J.H. Hampshire, V. Bellido, EU Patent EU 969249879 (1996).
 D.G. Teer, J. Hampshire, V. Fox, V. Bellido-Gonzalez, Surf. Coat. Technol. 94–95
 N.M. Renevier, H. Oosterling, U. König, H. Dautzenberg, B.J. Kim, L. Geppert, F.G.M.
Koopmans, J. Leopold, Surf. Coat. Technol. 172 (2003) 13.
 R.I. Amaro, R.C. Martins, J.O. Seabra, N.M. Renevier, D.G. Teer, Tribol. Int. 38 (2005)
 E. Arslan, F. Bülbül, A. Alsaran, A. Celik, I. Efeoglu, Wear 259 (2005) 814.
 M. Fenker, M. Balzer, H. Kappl, A. Savan, Surf. Coat. Technol. 201 (2006) 4099.
 N.M. Renevier, V.C. Fox, D.G. Teer, J. Hampshire, Surf. Coat. Technol. 127 (2000) 24.
 M.C. Simmonds, A. Savan, E. Pflüger, H. Van Swygenhoven, Surf. Coat. Technol. 126
 B.C. Stupp, Thin Solid Films 84 (1981) 257.
 G. Weise, A. Teresiak, I. Bacher, P. Markschlager, G. Kampsculte, Surf. Coat.
Technol. 76–77 (1995) 382.
 M.C. Simmonds, A. Savan, S.H. Van, E. Pfluger, S. Mikhailov, Surf. Coat. Technol.
108–109 (1998) 340.
 W.H. Kao, Y.L. Su, Mater. Sci. Eng. A 368 (2004) 239.
X. Ding et al. / Surface & Coatings Technology 205 (2010) 224–231
 X.Z. Ding, X.T. Zeng, Surf. Coat. Technol. 200 (2005) 1372.
 X.Z. Ding, X.T. Zeng, T. Goto, Surf. Coat. Technol. 198 (2005) 432.
 J.R. Lince, M.R. Hilton, A.S. Bommannavar, J. Mater. Res. 10 (1995) 2091.
 H. Mohrbacher, B. Blanpain, J.P. Celis, J.R. Roos, Wear 180 (1995) 43.
 K. Kato, Wear 241 (2000) 151.